- Open Access
Fabrication of naturel pumice/hydroxyapatite composite for biomedical engineering
- Baran Komur1Email authorView ORCID ID profile,
- Tim Lohse2, 12,
- Hatice Merve Can3, 4, 12,
- Gulnar Khalilova3, 12,
- Zeynep Nur Geçimli5,
- Mehmet Onur Aydoğdu6, 12,
- Cevriye Kalkandelen7,
- George E. Stan8,
- Yesim Muge Sahin9, 12,
- Ahmed Zeki Sengil10,
- Mediha Suleymanoglu11,
- Serap Erdem Kuruca11,
- Faik Nuzhet Oktar3, 12,
- Serdar Salman13,
- Nazmi Ekren12, 14,
- Anton Ficai15 and
- Oguzhan Gunduz12, 13
© The Author(s) 2016
- Received: 28 March 2016
- Accepted: 22 June 2016
- Published: 7 July 2016
We evaluated the Bovine hydroxyapatite (BHA) structure. BHA powder was admixed with 5 and 10 wt% natural pumice (NP). Compression strength, Vickers micro hardness, Fourier transform infrared spectroscopy, scanning electron microscopy (SEM) and X-ray diffraction studies were performed on the final NP-BHA composite products. The cells proliferation was investigated by MTT assay and SEM. Furthermore, the antimicrobial activity of NP-BHA samples was interrogated.
Variances in the sintering temperature (for 5 wt% NP composites) between 1000 and 1300 °C, reveal about 700 % increase in the microhardness (~100 and 775 HV, respectively). Composites prepared at 1300 °C demonstrate the greatest compression strength with comparable result for 5 wt% NP content (87 MPa), which are significantly better than those for 10 wt% and those that do not include any NP (below 60 MPa, respectively).
The results suggested the optimal parameters for the preparation of NP-BHA composites with increased mechanical properties and biocompatibility. Changes in micro-hardness and compression strength can be tailored by the tuning the NP concentration and sintering temperature. NP-BHA composites have demonstrated a remarkable potential for biomedical engineering applications such as bone graft and implant.
- Natural pumice
- Bovine hydroxyapatite
- Bioinspired composites
Worldwide, there is an estimated amount of 56 million bone fractures due to an increased life expectancy and thus the occurrence of age-related illnesses such as osteoporosis, a disease, which leads to a loss of bone mass . In the world, the lifetime risk of a bone fracture is 40–50 % for women and 13–22 % for men . Since life expectancy is on the rise all over the world, the frequency of such medical issues will only grow further. Hence, an expansion of the market for biomaterials that can be used in bone tissue engineering is to be expected. The financial impact of bone fractures is substantial; in the US alone the costs of bone fracture treatments for the health care system were situated in the range $12.2–$17.9 billion in 2002 . A reduction of such costs by finding new highly reliable but low-priced bone substitute materials has great potential benefits for society.
Today’s state-of-the-art bone substitute is synthetic hydroxyapatite [HA, Ca10(Po4)6(OH)2)] . Its composition is similar to the mineral constituent of bones or teeth . HA can be produced synthetically by various chemical routes such as: precipitation, hydrothermal method, hydrolysis of other calcium phosphates or sol–gel process .
However, HA can be also derived from bovine femur bones and it is already available as a commercial product under the Cerabone® and Endobon® trademarks .
Bovine femur bones show a micro-hardness which ranges between 47.92 ± 3.98 HV and 71.99 ± 8.97 HV. Bone is a nanocomposite constituted of HA nanocrystals (bone mineral sums up to ~70 wt% of the bone mass, the rest being collagen and other small amounts of proteins and inorganic salts) embedded in a matrix of collagen microfibrils . The bone hardness values differ with the orientation of HA crystallites-collagen microfibrils assembly. The more crystals are perpendicular to the measuring surface, the harder is . Human bone has a compressive strength of ~200 MPa .
Unlike bone, pure HA is a material with weak mechanical properties. The compressive strength ranges from 12 MPa (when sintered at 1000 °C and previously compressed at 350 MPa) to 64 MPa (at 1200 °C, 350 MPa). The micro-hardness ranges from 85 HV (at 1000 °C, 350 MPa) to 170 HV (at 1200 °C, 350 MPa) . Other sources report a micro-hardness ranging from 61 HV (when sintered at 1100 °C and previously compressed at 156 MPa) to 200 HV (at 1300 °C, 156 MPa) , and a compressive strength around 50 MPa (for 1200 and 1300 °C sintering temperatures) .
One method to improve the mechanical properties of HA is the incorporation of glass–ceramics derived from silica—or phosphate-based bioactive glasses. The result is a composite material with higher strength and improved biocompatibility . For example, the compressive strength of HA admixed with 2.5 wt% Na2O–CaO–P2O5 glass, sintered at 1200 °C, is 110 MPa .
In this study, natural pumice (NP)—a naturally occurring glass–ceramic of volcanic origin—was used to reinforce bovine-derived hydroxyapatite (BHA). NP is the product of lava being cooled and depressurised, e.g. when a volcanic eruption takes place. It occurs only when enough gases, such as H2O, CO2 and SO2, are dispersed in magma. The liquid magma melt can then transform into single fragments of foamy melt within the gas phase. This process is called magmatic fragmentation [16, 17]. It typically happens during plinian volcanic eruptions, which are characterised by a catapulting of mostly coarse particles (>1 mm) into the air using them in a relatively large area (ca. 1500 km2) around the volcano [18, 19]. NP is a highly porous material with a porosity of about 90 %, with all the porosity being interconnected. The pores are often of cylindrical shape, since the maximum packing density of a cylinder is higher than those of a sphere . The density of NP is 1.2–1.4 g/cm3 and its compressive strength is 1.72 ± 0.12 MPa . It is composed of mainly SiO2 (60–75 wt%), Al2O3 (13–17 wt%), Na2O–K2O (7–8 wt%) and smaller amounts of Fe2O3, TiO2 and CaO, etc. .
In-vitro testing of NP has shown good MG63 cell viability . As aforementioned, BHA is already in use for medical applications , but it offers only limited mechanical properties . However, previous studies with composites of HA and SiO2-based bioglass have shown promising results regarding both biocompatibility and mechanical strength [22, 24]. For example, HA has been reinforced with the SiO2-based 45S5 Bioglass® and sintered by using a heat-treatment program with a maximum temperature of 1000 °C, resulting in a higher strength . On the other hand, there are also studies that state that the addition of 2 wt% SiO2 to HA does not change the compressive strength , therefore it is suggested that the other alkali and alkali-earth oxides typical of bioglass formulations might play the prominent role in the improvement of the mechanical response. However, in vitro tests in simulated body fluids and osteogenic cell cultures demonstrated that a composite of HA with a silicate-based additive has greater bioactivity and biocompatibility than pure HA .
With all this in mind, it stands to reason to investigate a new composite material fabricated from sustainable resources such as natural pumice and bone derived hydroxyapatite. The aim of this study is to introduce a new bio-inspired composite (NP-BHA) eliciting biocompatibility and mechanically superior properties, thus suitable for bone reconstruction applications.
Composition of the natural pumice used in our experiments 
Preparation of NP-BHA
The natural pumice and bovine hydroxyapatite powders were grounded and sieved separately to achieve a mean grain size of ~100 µm. The HA powder was then mixed with 5 and 10 wt% of NP powder, respectively. The samples will be further denominated as 5 wt% NP-BHA and 10 wt% NP-BHA. Each mixture was then further grounded for 4 h in the ball mill. The samples were then prepared according to British standard 7253: The mixtures were compressed between two hardened steel bodies at 350 MPa. The resulting cylinders were then sintered at different temperatures (1000, 1100, 1200 and 1300 °C) for 4 h using a HT 16/17 furnace (Nabertherm GmbH, Lilienthal, Germany). The procedure used is according to previous research conducted by Gunduz et al. .
NP-BHA composite characterization
The morphology of the samples prior and after the in vitro testing was investigated by scanning electron microscopy (SEM), using a SEM JEOL 590, Tokyo, Japan. The bonding configuration and identification of functional groups was performed by Fourier Transform Infrared (FTIR) spectroscopy, using a Perkin Elmer Spectrum BX apparatus in attenuated total reflectance mode (1.8 diameter Pike-MIRacle Diamond Head). The spectra were collected over a range of 1800–550 cm−1 by recording 128 individual scans at a resolution of 4 cm−1. The identification of crystalline phases was made by X-ray Diffraction (XRD) using a Bruker D8 Advance diffractometer, with Cu Kα (λ = 1.5418 Å) radiation, equipped with a high efficiency linear detector of Lynx Eye type. The samples were measured in symmetric geometry in the angular range 2θ = 5°–60°, with 0.04° step size and 10 s acquisition time per step.
The compression test was conducted with a speed of 2 mm/min using the universal tensile testing machine DVT (Devotrans Inc., Istanbul, Turkey). The micro-hardness (HV) was tested with a load of 200 g and 20 s dwell time using the HMV-2 (Shimadzu, Kyoto, Japan). This procedure was carried out which are performed according to previous research .
Cytocompatibility of the samples (NP-BHA composites, as well as simple NP and BHA controls) was evaluated by culturing with primary human osteosarcoma cells (Saos-2) provided by the American Type Culture Collection (ATTC). The osteoblast-like Saos-2 cell line is widely used as an in vitro biocompatibility model for materials with bone regeneration applications [38, 39]. The cells were routinely grown in Dulbecco’s Modified Eagle Medium (DMEM) medium (Sigma Chemical, St. Louis, MO, USA) supplemented with 10 % volume fraction of calf serum (Gibco, Rockville, MD, USA), 100 UI/ml penicillin, 100 µg/ml streptomycin, and l-glutamine. Cells were subcultured once a week using trypsin and maintained at 37 °C in an incubator with humidified 5 % CO2 atmosphere. The medium was changed every 3 days. The confluent cells were used in cytotoxicity tests .
First, the conditioned medium was prepared to understand any possible toxic effect induced by possible ionic leach-out product from the samples into the medium. For this aim, 10 mL fresh medium was added in tubes with 1 g of tested material (NP-BHA composites, NP and BHA), which were kept in the incubator. One week after the conditioned medium was extracted, and later used in cytotoxicity tests.
The Saos-2 cells (105 cells per well) were seeded in 98-wells micro plate, conditioned medium and unconditioned DMEM medium as control, Plates were transferred to a humidified atmosphere incubator, and after 3 days the cell proliferation was measured by classic MTT test. The culture media were removed, and 10 uL (5 mg/ml) of MTT (Sigma Chemical, St. Louis, MO, USA) solution was added to each well. Following incubation at 37 °C for 4 h in a humidified 5 % CO 2 atmosphere, the media was discarded. The precipitated formazan was dissolved in dimethyl sulfoxide (150 µL per well), and optical density was evaluated using a micro plate spectrophotometer at a wavelength of 570 nm.
The cytotoxicity assays were conducted in triplicate. A t test was performed to determine the statistical significance between experimental groups. Kruskal–Wallis test was used to compare the groups. A value of p <0.05 was considered to be statistically significant.
Each specimen (5.0 mm in diameter and 1.0 mm in length) was sterilized with 96 % ethanol and ultraviolet radiation. After washing the samples with medium, they were put in wells with 5 mL of fresh medium (without cells), and kept overnight in incubator. Saos-2 cells were seeded on the surface of pre-wetted specimens (10 × 105 cells per specimen). The specimens were then placed in 6-wells cell culture plates, and maintained for 3 h in incubator to allow the cells to attach. Then, additional 1 mL culture medium was added into each well, and transferred into the incubator. The medium was changed at 2 days. After 4 days, the media were removed, and the cells were fixed with 3 % volume fraction of glutaraldehyde, subjected to graded alcohol dehydration, rinsed with isoamyl acetate, and observed by a scanning electron microscopy.
Antimicrobial activity evaluation
First, antimicrobial activity of NP and NP-BHA samples was determined by using a qualitative diffusion disk test method . Enterococcus faecalis ATCC 29212, Staphylococcus aureus ATCC 6538 and Escherichia coli ATCC 25922 strains were used as test microorganisms in this study. The test strains (105 CFU/mL) were inoculated on MHA (Muller Hinton Agar) surface using Drigalsky loop. The NP and NP-BHA pellets of 10 mm in diameter were positioned at the centre of the Petri plates. The plates were incubated at 37 °C up to 24 h. The microbial inhibition zones on the samples’ surface were evaluated at 6 and 24 h.
A quantitative analysis for the confirmation of antimicrobial activity of NP and NP reinforced materials against E. faecalis ATCC 29212 strain has been performed. Powdered specimens were added to 9 mL Muller Hinton broth to final concentration of 10 mg/mL. Enterococcus faecalis test strain (104–105 CFU/mL) was added and specimens incubated at 37 °C for 24 h. 1 mL sample was taken from this mixture and analysed by spectrophotometry for microbial counts at the 0, 6 and 24 h. The analyses were performed in triplicate.
The sintering treatment performed at 1100 °C hinted towards a continuous transformation of HA into β-TCP with temperature (Fig. 5b), and also induced the increase in crystallinity of the Ca2Al(AlSi)O7 and Ca5(PO4)2SiO4 phases. If in the case of 5 wt% NP-BHA sample, BHA is still the prominent constituent, whilst the 10 wt% NP-BHA material is now dominated by β-TCP, with HA as a secondary phase.
After the 1200 °C sintering, the β-TCP content increases for both 5 and 10 wt% NP-BHA composites (Fig. 5c). If in the case of 5 wt% NP-BHA, the Ca5(PO4)2SiO4 reaches its zenith in terms of crystallinity, in the case of 10 wt% NP-BHA the calcium phosphate silicate phase peaks seem less prominent and the emergence of a new phase—α-SiO2 (ICDD: 01-080-2148)—is now detected.
The sintering treatment performed at 1300 °C induced radical structural modifications (Fig. 5d). Interestingly, the diffraction pattern of the 5 wt% NP-BHA sample indicated only the presence of hydroxyapatite along two new minor phases: CaNaAlSi2O7 (ICDD: 01-071-2066) and (Ca2.87Fe0.13)(Al1.9Fe0.1)(SiO4)3 (ICDD:01-085-1508). The β-TCP and Ca2Al(AlSi)O7 phase are now absent, whilst the intensity of the Ca5(PO4)2SiO4 diffraction lines diminished in comparison with the 5 wt% NP-BHA sample sintered at 1200 °C. On the other hand, the 10 wt% NP-BHA diffractogram indicated the total decomposition of BHA and the partial transformation of the low-temperature polymorph β-TCP into the high-temperature polymorph α-TCP (ICDD: 00-003-0681). Also, after the sintering treatment performed at 1300 °C, the diffraction lines of 10 wt% NP-BHA are broader, whilst their intensity is significantly reduced. The presence of Ca5(PO4)2SiO4 is still noticeable, along the newly emerged (Ca2.87Fe0.13)(Al1.9Fe0.1)(SiO4)3 phase.
The thermal decomposition of BHA is accompanied by an overall decrease in intensity of the diffraction lines and their broadening. The regular line shifts recorded for both BHA and β-TCP phases during sintering, with respect to the reference ICDD file positions, advocate for the occurrence of various lattice ionic substitutions with the species appertaining to the reinforcing NP agent.
The XRD results also suggest a dependency of the decomposition rate of BHA on the mass fraction of NP within the composites. One can observe that, in the case of 5 wt% NP-BHA, the BHA transformation into TCP takes place at a slower pace than in the case of 10 wt% NP-BHA. The driving force of BHA decomposition is given by its gradual dehydration with increasing sintering temperature . After the release of water molecules from the HA structure, a dehydrated unstable and faulty lattice is created, which is highly susceptible to both chemical reactions, ionic substitutions from surrounding media, and thereby decomposition or nucleation of new phases. In such a case, the amount of reinforcing compound in the composite will play a decisive role on the BHA decomposition speed at a given temperature, as the hydroxyl loses during sintering can be compensated by various chemical species of pumice found in intimate contact with BHA. The different thermal expansion coefficients of BHA and NP crystalline phases can also induce high stresses at the grain boundaries and enhance the thermal decomposition of the BHA phase .
The TCP conversion to BHA at elevated temperatures is not unprecedented . Kong et al. have stated that at high temperatures the Ca ions from the HA regions have the ability to diffuse into the β-TCP regions and convert the TCP into a Ca-deficient HA .
Our results seem to indicate that such a phenomenon can occur only if a larger concentration of BHA should pre-exist in a given sample, such as the case of 5 wt% NP-BHA (Fig. 5c vs. d). If the β-TCP is the dominant phase in the composite, the sintering will lead to a further decomposition of BHA, and eventually to the β-TCP transformation into its high-temperature polymorph, α-TCP (Fig. 5c vs. d).
Few other additional vibration bands, with maxima at 804, 881, 1421, 1457, 1483, and 1512 cm−1, can be noticed in the BHA powder spectrum (Fig. 6c), which emphasize the biological origin of this material. The presence of absorption bands at 881, 1421, 1457, 1483, and 1512 cm−1 is attributed to the ν2 bending and ν3 stretching modes of carbonate (CO3)−2 groups, and indicate a AB-type double substitution into the HA lattice: (i) substitution of OH− with (CO3)−2 (A-type substitution) and ii) substitution of (PO4)−3 with (CO3)−2 (B-type substitution) due to charge compensation necessity The weak band at 881 cm−1 can be also the result of the overlapping of the vibration band of (HPO4)−2 with the ν2 bending mode of carbonate The existence in bone mineral of ions in non-apatitic domains has been documented in the past and it is usually located in a hydrated layer on the surfaces of the apatitic crystals Such a layer is known to contain prevalently bivalent ions such as HPO4)−2 and (CO3)−2 The peak at 804 cm−1 advent from the OH− deformation band of BHA structure .
The IR spectrum of NP is dominated by a main broad peak centred at 989 cm−1, having two additional side shoulders positioned at 877 and 1134 cm−1 (Fig. 6d). The bands can be assigned to the characteristic vibrations of silicate groups. The bands’ broadening is consistent with a less-ordered structure. The band at 1134 cm−1 can be ascribed to the ν3 asymmetric stretching vibration of Si–O–Si bonds The band centred at 989 cm−1 evidences by the asymmetric stretching vibrations of Si–O–Al bonds The faint band peaking at 877 cm−1 can be attributed to the SiO4 units with non-bridging oxygen atoms (most probably Q3 and Q2 units) . The other vibrational bands located on the low wave numbers region unveiled the typical symmetric stretching (714, 772 cm−1), bending (635 cm−1) and rocking (578 cm−1) vibrational modes of various silicate groups The shift of IR bands to low wavenumbers is generated by incorporation of Al3+ into the Si4+ sites and the structural modifications determined by the breaking of oxygen bridges due to the presence of the alkali and alkali-earth species, and consequently their charge compensation necessity. Such phenomena are prone to take place as the excess negative charge arising from the Al3+→ Si4+ replacement might not be enough to balance the positive ions (alkali and alkali-earth cations) charge, which are presented in NP and sum up to ~11 wt% of its composition.
The Q2, Q1, and Q0 phosphate units yield IR vibration bands in the 1400–400 cm−1 range However, the vibrations of phosphate groups present in NP are difficult to be emphasized because of the low P content of the material and the superimposition of prominent of silicate units in the fingerprint absorption region. The presence of the ν3 asymmetric stretching lines of (CO3)−2 (~1440 cm−1) and bending vibrations of adsorbed water molecules (1639 cm−1) were also evidenced. We stress that the 877 cm−1 peak can be associated only partially to the ν2 bending of carbonate, as the intensity of such a vibration mode is considered to be only ~1/5 of the ν3 asymmetric stretching band of carbonate .
Both low (Fig. 7a, b) and high (Fig. 7c, d) wavenumbers regions of the composites are dominated by vibrational bands of phosphate functional groups. The more intricate IR envelops of 10 wt% NP-BHA composite with respect to the one of 5 wt% NP-BHA sample, at every sintering temperature, support the higher rate and degree of BHA decomposition. Due to the aforementioned coexistence in the same spectral regions of the phosphate and silicate vibrational mode, the NP bands are more difficult to be unravelled.
The triply degenerated bands of ν3 asymmetric stretching mode (1011/1012, 1023/1024 and 1087/1086 cm−1), and of the ν4 bending mode (556/555, 565/565 and 599/600 cm−1), as well as of the ν1 symmetric stretching (962/962 cm−1), evidenced in the 5 and 10 wt% NP-BHA composites, belong to the structural vibrations of phosphates groups in both BHA and β-TCP (Fig. 7a, b).
One can notice that the libration band of structural OH− units of BHA (Fig. 7a, c vs. a, b) is reducing progressively with the increase of sintering temperature. The process is more acute in the case of 10 wt% NP-BHA composite. As stated before (see XRD chapter), the dehydration of HA plays a prominent role in its decomposition kinetics. As a consequence the phosphate functional groups enter a restructuring process, which is clearly illustrated by FTIR spectra (Fig. 7).
The bands positioned at 944/947 and 982/982 cm−1 are distinctive to a β-TCP phase and are present for both composites after the sintering treatment at 1000 °C. The 1121 cm−1 shoulder is present in the 10 wt% NP-BHA (Fig. 7d) after the 1000 °C sintering, and appears (at 1120 cm−1) for 5 wt% NP-BHA (Fig. 7c) only after a sintering treatment performed at a higher temperature (1100 °C), and disappears after the 1300 °C sintering in the case of both types of composites. The band is typical for a β-TCP heated at temperatures ≥1000 °C , and its evolution with increasing sintering temperature correlates well with the gradual decrease of the libration band of structural OH− units. Thus, the FTIR results are in good agreement with the XRD findings, which suggested that the BHA lattice dehydroxylation allows for the structuring of the β-TCP counterpart.
The new shallow shoulder emerging at 883/888 cm−1 after the sintering at 1200 °C for both composites (Fig. 7c, d) could be ascribed to the increase of short-range order of silicate based compounds, whose presence was confirmed by the XRD results (Fig. 6). After the sintering at 1300 °C, significant modifications were recorded in the IR spectra of NP-BHA composites. The 5 wt% NP-BHA exhibits only the bands of the triply degenerated ν3 asymmetric stretching and ν4 bending modes together with ones of the ν1 symmetric stretching. The absence of the libration band of hydroxyl groups (Fig. 7c) suggests the formation of an oxyapatite compound, in good agreement with the XRD observations (Fig. 5). In the case of the 10 wt% NP-BHA (Fig. 7d) the bands became broaden hinting towards a dramatic structural transformation, whilst the characteristic bands of β-TCP (947, 982 and 1121 cm−1) are still present, but their intensity is more reduced.
Figure 8b the compressive strength values recorded in the case of NP-BHA composites. For sintering temperatures above 1100 °C, the 5 wt% NP-BHA composite elicited higher compressive strength values. Only when applying a sintering temperature of 1000 °C, the 10 wt% NP-BHA composite was stronger than the 5 wt% NP-BHA composite, most probably due to more decreased porosity (see Fig. 1). The highest compressive strength (87 ± 0.5 MPa) was recorded for 5 wt% NP-BHA composite sample sintered at 1300 °C. This is an improvement compared to the 12–64 MPa of pure HA which thus demonstrate the positive reinforcing effect of natural pumice.
Compared to common bone substitute materials, such as tricalcium phosphate (compressive strength: 10.95 ± 1.28 MPa) or commercially available products like Calcibon® (35–55 MPa), Norian SRS® (23–55 MPa) and HydroSet® (14–24 MPa)  the NP-BHA composite introduced in the present study has a significantly higher compressive strength. However, it does not meet yet the average compressive strength of human cortical bone, which varies between 100–150 MPa . Goller et al.  have added reduced quantities of bioglass (5 and 10 wt%) to BHA to prepare composite structures. The best compression result (~83 MPa) was achieved at a sintering temperature of 1200 °C in the case of the 10 wt% bioglass reinforced material. Thus, a direct comparison shows that the 5 wt% NP reinforced BHA material demonstrated a slightly higher compression value (~87 MPa).
Antimicrobial activity of natural pumice and NP-BHA composites
5 wt% NP-BHA
10 wt% NP-BHA
6.7 × 104
7.4 × 104
7.0 × 104
5.6 × 104
8.3 × 107
9.8 × 107
8.3 × 107
1.1 × 108
5.0 × 108
1.3 × 109
3.0 × 108
1.8 × 109
We have successfully synthesized new biocompatible materials, based on cheap sustainable resources [bovine hydroxyapatite (BHA) and natural pumice (NP)], by powder pressing followed by sintering at temperatures in the range of 1000–1300 °C. A synergistic effect, in terms of both cytocompatibility and mechanical performance, has been recorded for the BHA composites reinforced with 5 wt% NP. Their in vitro biocompatibility behaviour was higher than that of pure BHA. Changes in micro-hardness and compression strength can be tailored by the tuning the NP concentration and sintering temperature. NP-BHA composites have demonstrated a remarkable potential for biomedical engineering applications such as bone graft and implant.
BK carried out the preparations and participated in the design of the manuscript. TL carried out the preparation and participated in the sequence alignment and drafted the manuscript. HMC helped in preparation, assessment of the materials and participated in the sequence alignment and drafted the manuscript. GK carried out the preparation and coordination and helped to draft the manuscript. ZNG participated in its design and coordination. MOA participated in the design of the study. CK participated in its design and coordination and helped to draft the manuscript. GES participated in the design of the study. YMS helped in preparation and assessment of the materials. AZS participated in its design and coordination and helped to draft the manuscript MS conceived of the study, and participated in its design and coordination and helped to draft the manuscript. SEK Participated in its design and coordination and helped to draft the manuscript. FNO conceived of the study and coordination and helped to draft the manuscript. SS helped to draft the manuscript. NE participated in its design and coordination and helped to draft the manuscript. AF helped to draft the manuscript and editing. OG conceived of the study and editing. All authors read and approved the final manuscript.
Financial support of Marmara University, Istanbul, Turkey, through research projects FEN-B-080415-0117 and FEN-C-YLP-140115-0008 is acknowledged. GES is thankful for the financial support of the NIMP PN4501-3 Core Programme.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Johnell O, Kanis JA. An estimate of the worldwide prevalence and disability associated with osteoporotic fractures. Osteoporos Int. 2006;17:1726–33.View ArticleGoogle Scholar
- Johnell O, Kanis JA. Epidemiology of osteoporotic fractures. Osteoporos Int. 2005;16:3–7.View ArticleGoogle Scholar
- DeJesus RS, Angstman KB, Kesman R, Stroebel RJ, Bernard ME, Scheitel SM, Chaudhry R. Use of a clinical decision support system to increase osteoporosis screening. J Eval Clin Pract. 2012;18(1):89–92.View ArticleGoogle Scholar
- Arafat MT, Gibson I, Li X. State of the art and future direction of additive manufactured scaffolds based bone tissue engineering. Rapid Prototyp J. 2014;20:13–26.View ArticleGoogle Scholar
- Lahiri D, Ghosh S, Agarwal A. Carbon nanotube reinforced hydroxyapatite composite for orthopedic application: a review. Mater SciEng C. 2012;32:1727–58.View ArticleGoogle Scholar
- Seidel P, Dingeldein E. Cerabone®—einespongiosa-keramikbovinenursprungs. Mat-wissWerkstofftech. 2004;35(4):208–12.View ArticleGoogle Scholar
- Tadic D, Epple M. A thorough physicochemical characterisation of 14 calciumphosphate-based bone substitution materials in comparison to natural bone. Biomaterials. 2004;25:987–94.View ArticleGoogle Scholar
- Koutsopoulos S. Synthesis and characterization of hydroxyapatite crystals: a review study on the analytical methods. J Biomed Mater Res. 2002;62(4):600–12.View ArticleGoogle Scholar
- Ziv V, Wagner HD, Weiner S. Microstructure-microhardness relations in parallel-fibered and lamellar bone. Bone. 1996;18(5):417–28.View ArticleGoogle Scholar
- Carter DR, Hayes WC. Bone compressive strength: the influence of density and strain rate. Science. 1976;194:1174–6.View ArticleGoogle Scholar
- Gunduz O, Gode C, Ahmad Z, Gökçe H, Yetmez M, Kalkandelen C, Sahin YM, Oktar FN. Preparation and evaluation of cerium oxide-bovine hydroxyapatite composites for biomedical engineering applications. J Mech Behav Biomed. 2014;35:70–6.View ArticleGoogle Scholar
- Herliansyah MK, Hamdi M, Ide-Ektessabi A, Wildan MW, Toque JA. The influence of sintering temperature on the properties of compacted bovine hydroxyapatite. Mater Sci Eng C. 2009;29:1674–80.View ArticleGoogle Scholar
- Rámila A, Padilla S, Munoz B, Vallet-Regí MA. New hydroxyapatite/glass biphasic material: in vitro bioactivity. Chem Mater. 2002;14:2439–43.View ArticleGoogle Scholar
- Georgiou G, Knowles JC. Glass reinforced hydroxyapatite for hard tissue surgery—part 1: mechanical properties. Biomaterials. 2001;22:2811–5.View ArticleGoogle Scholar
- Santos JD, Reis RL, Monteiro FJ, Knowles JC, Hastings GW. Liquid phase sintering of hydroxyapatite by phosphate and silicate glass additions: structure and properties of the composites. J Mater Sci Mater Med. 1995;6(6):348–52.View ArticleGoogle Scholar
- Manville V, White JDL, Houghton BF, Wilson CJN. The saturation behaviour of pumice and some sedimentological implications. Sediment Geol. 1998;119:5–16.View ArticleGoogle Scholar
- Gardner JE, Thomas RME, Jaupart C, Tait S. Fragmentation of magma during plinian volcanic eruptions. Bull Volcanol. 1996;58(2–3):144–62.View ArticleGoogle Scholar
- Walker GPL. Explosive volcanic eruptions—a new classification scheme. GeolRundsch. 1973;62(2):431–46.Google Scholar
- Li X, Yang W, Zou Q, Zou Y. Investigation on microstructure, composition, and cytocompatibility of natural pumice for potential biomedical application. Tissue EngPt C. 2010;16–3:427–34.View ArticleGoogle Scholar
- Pattan JN, Mudholkar AV, Sankar SJ, Ilangovan D. Drift pumice in the central indian ocean basin: geochemical evidence. Deep Sea Res Pt I. 2008;55:369–78.View ArticleGoogle Scholar
- Turhan Ş, Gündüz L. Determination of specific activity of 226Ra, 232Th and 40 K for assessment of radiation hazards from Turkish pumice samples. J Environ Radioactiv. 2008;99:332–42.View ArticleGoogle Scholar
- Zakaria SM, Zein SHS, Othmann MR, Yang F, Jansen JA. Nanophase hydroxyapatite as a biomaterial in advanced hard tissue engineering: a review. Tissue Eng Pt B. 2013;19(5):431–41.View ArticleGoogle Scholar
- Belluci D, Sola A, Gazzarri M, Chiellini F, Cannillo V. A new hydroxyapatite-based biocomposite for bone replacement. Mater SciEng C. 2013;33:1091–101.View ArticleGoogle Scholar
- Santos JD, Knowles JC, Reis RL, Monteiro FJ, Hastings GW. Microstructural characterization of glass-reinforced hydroxyapatite composites. Biomaterials. 1994;15(1):5–10.View ArticleGoogle Scholar
- Kivitz E, Görke R, Schilling AF, Zhang J, Heinrich JG. Influence of processing parameters on microstructure and biocompatibility of surface laser sintered hydroxyapatite–SiO2 composites. J Biomed Mater Res Part B. 2013;101(4):568–75.View ArticleGoogle Scholar
- Mossman NT. Rapid colorimetric assay for cellular growth and survivals: application to proliferation and cytotoxicity assays. J Immunol Methods. 1983;65:55–63.View ArticleGoogle Scholar
- Díaz M, Barba F, Miranda M, Guitián F, Torrecillas R, Moya JS. Synthesis and antimicrobial activity of a silver-hydroxyapatite nanocomposite. J Nanomaterials. 2009;14.Google Scholar
- Mestres G, Le Van C, Ginebra MP. Silicon-stabilized α-tricalcium phosphate and its use in a calcium phosphate cement: characterization and cell response. Acta Biomater. 2012;8(3):1169–79.View ArticleGoogle Scholar
- Evans EJ, Inglethorpe SDJ, Wetton PD. Mineralogy and Petrology Group, British Geological Survey, Technical report (WG/99/015). Nottingham; 1999.Google Scholar
- Barralet J, Knowles JC, Best S, Bonfield W. Thermal decomposition of synthesised carbonate hydroxyapatite. J Mater Sci Mater Med. 2002;13:529–33.View ArticleGoogle Scholar
- Cihlář J, Buchal A, Trunec M. Kinetics of thermal decomposition of hydroxyapatite bioceramics. J Mater Sci. 1999;34:6121–31.View ArticleGoogle Scholar
- Yang C, Guo YK, Zhang ML. Thermal decomposition and mechanical properties of hydroxyapatite ceramic. Trans Nonferrous Met Soc China. 2010;20:254–8.View ArticleGoogle Scholar
- Kong YM, Kim HE, Kim HW. Phase conversion of tricalcium phosphate into Ca-deficient apatite during sintering of hydroxyapatite-tricalcium phosphate biphasic ceramicsJ. Biomed Mater Res B. 2008;84:334–9.View ArticleGoogle Scholar
- Voltolini M, Wenk HR, Gomez Barreiro J, Agarwal SC. Hydroxylapatite lattice preferred orientation in bone: a study of macaque, human and bovine samples. J Appl Crystallogr. 2011;44:928–34.View ArticleGoogle Scholar
- Markovic M, Fowler BO, Tung MS. J Res Nat Inst Stand Technol. 2004;109:553–68.View ArticleGoogle Scholar
- Smolen D, Chudoba T, Malka I, Kedzierska A, Lojkowski W, Swieszkowski W, Kurzydlowski KJ, Kolodziejczyk-Mierzynska M, Lewandowska-Szumiel M. Highly biocompatible, nanocrystalline hydroxyapatite synthesized in a solvothermal process driven by high energy density microwave radiation. Int J Nanomed. 2013;8:653–68.View ArticleGoogle Scholar
- Miculescu F, Stan GE, Ciocan LT, Miculescu M, Berbecaru A, Antoniac I. Cortical bone as resource for producing biomimetic materials for clinical use. Digest J Nanomater Biostruct. 2012;7:1667–77.Google Scholar
- Socrates G. Infrared and Raman Characteristic Group frequencies—tables and charts. Hoboke: John Wiley & Sons Ltd; 2007.Google Scholar
- Berzina-Cimdina L, Borodajenko N. Research of calcium phosphates using fourier transform infrared spectroscopy, infrared spectroscopy—materials Science, engineering and technology. In: Theophile T editor. Rijeka: InTech; 2012.Google Scholar
- Oktar FN, Agathopoulos S, Ozyegin LS, Gündüz O, Demirkol N, Bozkurt Y, Salman S. Mechanical properties of bovine hydroxyapatite (BHA) composites doped with SiO2, MgO, Al2O3, and ZrO2. J Mater Sci Mater Med. 2007;18:2137–43.View ArticleGoogle Scholar
- Gunduz O, Ahmad Z, Ekren N, Agathopoulos S, Salman S, Oktar FN. Reinforcing of biologically derived apatite with commercial inert glass. J Thermoplas Comp Mater. 2009;22:407–19.View ArticleGoogle Scholar
- Banerjee SS, Tarafder S, Davies NM, Bandyopadhyay A, Bose S. Understanding the influence of MgO and SrO binary doping on the mechanical and biological properties of β-TCP ceramics. Acta Biomater. 2010;6(10):4167–74.View ArticleGoogle Scholar
- Fu Q, Saiz E, Rahaman MN, Tomsia AP. Bioactive glass scaffolds for bone tissue engineering: state of the art and future perspectives. Mater Sci Eng C. 2011;31:1245–56.View ArticleGoogle Scholar
- Goller G, Demirkıran H, Oktar FN, Demirkesen E. Processing and characterization of bioglass reinforced hydroxyapatite composites. Ceram Int. 2003;29:721–4.View ArticleGoogle Scholar